Download  Acidity of twodimensional zeolites
This journal is© the Owner Societies 2015 Phys. Chem. Chem. Phys., 2015, 17, 2787327882  27873
Cite this:Phys.Chem.Chem.Phys.,
2015, 17, 27873
Acidity of twodimensional zeolites†
Marcin Rybicki and Joachim Sauer*
Hybrid quantum mechanics:molecular mechanics (QM/MM) calculations of absolute deprotonation
energies are performed with periodic boundary conditions for Brønsted sites of aluminosilicate bilayers
with various Al/Si ratios (twodimensional zeolite). The supercell method is applied and density
functional theory is used. Much lower values are obtained (1042, 1069 and 1091 kJ mol�1 for Al/Si = 1/63,
1/7 and 1/3, respectively) than those for bulk zeolites (1233 kJ mol�1 for Hchabazite with Al/Si = 1/11).
We ascribe the much lower deprotonation energy to the smaller effective dielectric constant (1.6–1.9)
of an ultrathin dielectric in a vacuum compared to that of the corresponding bulk systems (3.0 for
Hchabazite), which leads to a better stabilization of the charge created upon deprotonation.
1. Introduction
Zeolites are crystalline porous aluminosilicates which are naturallyoccurring or synthesized. They are widely used as catalysts inindustrial processes such as catalytic cracking of crude oil,methanol to gasoline conversion and olefin oligomerization.1,2
The catalytic activity of proton forms of zeolites originates frombridging Al–O(H)–Si groups which represent Brønsted acid sites.3,4
In recent years a particular class of materials, twodimensionalzeolites, has attracted interest.5 They exist either as nanosheets,as thin as single unit cells of, e.g. MFI,6,7 or as ultrathin modelsystems grown under UHV conditions on metal substrates.8,9 Thelatter were prepared by the deposition of O2, Si and Al on theRu(0001) surface and subsequent adsorption and desorptionof water.8,9 They consist of an aluminosilicate bilayer with atwodimensional arrangement of hexagonal prisms and containsurface Brønsted sites.8 Thus, they may be considered astwodimensional zeolites (H2dH) with the flat surface corresponding to the infinite pore size.9 The advantage of the H2dHthin films is that their properties can be analysed using surfacescience techniques.
Adsorption of the weak bases CO and C2H2 on the acidic siteof the H2dH zeolite causes a red shift of the O–H stretchingband that is considerably higher than the shift observed for thebulk HSSZ13 zeolite, the protonated form of Hchabazite(HCHA).8,9 This suggests that the twodimensional (2D) zeolitestructures are considerably more acidic than the threedimensional(3D) ones.
The OH frequency shift upon adsorption of probe molecules10
is only one of the different measures of acidity strength.11–13 It isa reactivity parameter that assumes an ‘‘early’’ transition state. Incontrast, adsorption of strong bases like ammonia or pyridinethat have also been studied for H2dH and HCHA catalysts9
implies a late transition state with the proton being transferred tothe reaction partner. However, the heat of ammonia adsorptiondepends on two factors, the intrinsic acidity of the Brønsted site(which is larger for the 2D zeolite) and the van der Waalsinteraction between the ammonium ion formed and the surface.The latter is larger for the curved surface of the porous materialwhich is due to a better fit. A parameter that describesthe intrinsic acidity without any interaction between the basemolecule and the surface is the deprotonation energy (or theproton affinity of the deprotonated Brønsted site).4
The energy of adsorption, DEads, for the formation of aninteracting ion pair
Z–OH + B  Z–O�HB+ (1)
can be decomposed into the energy of the interaction,DEIP, between the protonated species and the deprotonatedsurface site,
Z–O� + HB+  Z–O�HB+ (2)
the deprotonation energy, DEDP, of the Brønsted site,
Z–OH  Z–O� + H+ (3)
and the proton affinity, DEPA, of the base molecule
B + H+  HB+ (4)
Hence,
DEads = DEIP + DEDP + DEPA (5)
Institut fur Chemie, HumboldtUniversitat zu Berlin, Unter den Linden 6,
10099 Berlin, Germany. Email: [email protected]
† Electronic supplementary information (ESI) available: Unit cell parameters,geometric parameters, figures of cluster models, and additional results fordeprotonation energies as well as x, y, and z coordinates for selected structures.See DOI: 10.1039/c5cp05088j
Received 26th August 2015,Accepted 14th September 2015
DOI: 10.1039/c5cp05088j
www.rsc.org/pccp
PCCP
PAPER
Ope
n A
cces
s A
rtic
le. P
ublis
hed
on 0
6 O
ctob
er 2
015.
Dow
nloa
ded
on 3
0/11
/201
5 10
:49:
30.
Thi
s ar
ticle
is li
cens
ed u
nder
a C
reat
ive
Com
mon
s A
ttrib
utio
n 3.
0 U
npor
ted
Lic
ence
.
View Article OnlineView Journal  View Issue
27874  Phys. Chem. Chem. Phys., 2015, 17, 2787327882 This journal is© the Owner Societies 2015
For molecules in the gas phase measuring the deprotonationenergy (or the proton affinity) is a wellestablished technique.Mass spectrometry yields proton transfer equilibrium constantsthat are converted into gas phase acidity and gas phase basicityscales, e.g., ref. 14. For surface hydroxyl groups, however,quantum chemical calculations are the only source.4,11,15,16
The aim of this work is to determine the intrinsic acidity ofH2dH zeolites by performing hybrid QM/MM calculations ofthe deprotonation energy, and to compare it with that of HCHAas an example of bulk zeolites. We also investigate the influenceof the Al/Si ratio on the acidity of the H2dH system and weanalyse the structure factors determining the deprotonationenergies.
2. Methods2.1 Periodicity and deprotonation energies
Zeolites are crystalline materials and theoretical investigationsof their properties have to take into account the periodicity ofthe system. The deprotonation energy of a zeolite (DEDP)is defined as the energy difference between the deprotonated(Z–O�) and the protonated (Z–OH) zeolite:
DEDP = EZO� � EZOH = DEvDP + Erel (6)
Using the energy of the deprotonated system ‘‘at the structureof’’ the parent system, EZO�//ZOH, it may be decomposed intoa ‘‘vertical’’ deprotonation energy, DEv
DP, and a relaxationenergy, Erel,
Erel = EZO� � EZO�//ZOH (7a)
DEvDP = EZO�//ZOH � EZOH (7b)
Applying periodic boundary conditions to the deprotonationprocess implies that a negative charge is created in every unitcell. This causes divergence of the electrostatic energy for thedeprotonated system, ZO�. It is also an unrealistic modelbecause in the catalytic process we do not expect release of aproton in every unit cell at the same time. The divergence of theelectrostatic energy can be eliminated by adding a uniformbackground charge to the deprotonated unit cell. The spuriousinteraction between the charged defects can be reduced usingthe supercell method or approximately eliminated using themethod proposed by Leslie and Gillan (LG method).17
2.1.1 The supercell approach. This is the simplest, butcomputationally most demanding method. We build a seriesof supercells by multiplying the original unit cell N times inevery direction and calculate the deprotonation energy for eachsupercell. We remove only one proton per supercell. Thisway, the distance between charged defects increases, and theartificial anion–anion interaction decreases. The deprotonationenergy of the zeolite becomes a function of N. In the limitof infinitely large N, its value, DEN
DP, is interpreted as thedeprotonation energy needed to remove the proton from anisolated Brønsted site. In the N � N � N supercell, the cubic
root of the supercell volume,ffiffiffiffiV3p
, can be defined as the averagedistance between the charged defect and its nearest periodic
images, hr��i. The deprotonation energy of the system can beextrapolated using the following equation:
DEDPðNÞ ¼ DE1DP þA
r��h i þB
r��h i3 ¼ DE1DP þ Ecorr (8)
where DEDP(N) is the deprotonation energy for the N � N � Nsupercell, and A and B are fitting parameters. The 1/r and 1/r3
terms of the total correction, Ecorr, correspond to charge–chargeand dipole–dipole interactions, respectively, and the parameters A and B reflect the screening properties of the material.
2.1.2 Aperiodic correction. The method proposed by Leslieand Gillan17 relies on the macroscopic approximation. Itassumes that the difference between the energy per unit cellfor the periodic defect and for the isolated defect is equal to theinteraction of a periodic array of point charges, E��, immersedin a dielectric medium with the dielectric constant e of thesystem without defects. Therefore, the deprotonation energycan be expressed as:
DELGDP ¼ DEDP �
E��eðLGÞ (9)
In practice, E�� is the energy of the point charge (usually H+)placed in the unit cell of the investigated system immersed inthe compensating background charge, whereas e(LG) is 1/3of the trace of the static dielectric tensor of the system.Comparison of eqn (8) and (9) shows that, if both correctionmethods are correct, the relationship:
E��e¼ A
r��h i þB
r��h i3 (10)
holds, from which we can calculate an effective dielectricconstant eeff(SC) from given A and B parameters. The Leslie–Gillan approach is valid if the original unit cell is big enough toencapsulate the structural deformation induced by the chargeddefect and the dielectric constant of the material is isotropic.Both conditions are usually fulfilled for bulk zeolites, and theLeslie–Gillan method of aperiodic correction is the method ofchoice for these materials.
2.2 Embedded cluster QM/MM calculations
To calculate the deprotonation energy of zeolites, we useda mechanical embedding scheme,18,19 which partitions thesystem (S) into the inner region (I) and the outer region (O).The dangling bonds of the inner part are saturated withhydrogen link atoms, and the inner part together with the linkatoms forms the cluster (C). The total energy E(S) and the forces
Fa(S) acting on the atoms are obtained as follows:18,19
E(S) = EQM(C) + EMM(S) � EMM(C) (11a)
Fa(S) =
Fa,QM(C) +
Fa,MM(S) � 
Fa,MM(C) a A I (11b)
Fb(S) =
Fb,MM(S) b A O (11c)
To the quantum mechanical results for the cluster, EQM(C) and
Fa,QM(C), the results of the periodic description of the lattice bythe force field, EMM(S) and

Fa,MM(S), are added. The thirdcontribution EMM(C) and

Fa,MM(C) eliminates approximately
Paper PCCP
Ope
n A
cces
s A
rtic
le. P
ublis
hed
on 0
6 O
ctob
er 2
015.
Dow
nloa
ded
on 3
0/11
/201
5 10
:49:
30.
Thi
s ar
ticle
is li
cens
ed u
nder
a C
reat
ive
Com
mon
s A
ttrib
utio
n 3.
0 U
npor
ted
Lic
ence
.View Article Online
This journal is© the Owner Societies 2015 Phys. Chem. Chem. Phys., 2015, 17, 2787327882  27875
the double counting of the contributions coming from atoms inthe inner region and artificial contributions from link atoms.For an atom a of the inner region, all three terms contribute tothe force acting on it. For an atom b of the outer region, theforce is obtained from the force field alone. A link atom is notmoved according to the force acting on it. It is instead fixed onthe bond which it terminates.19,20
If we apply the QMPot embedding scheme (eqn (11a))to calculate the zeolite deprotonation energy and introducethe notation CH, SH, C� and S�, for the cluster C and thetotal system S of the protonated and deprotonated form,respectively, we obtain:
DEDP = DEDP(QM) + DEDP(MM) (12a)
with:
DEDP(QM) = EQM(C�) � EQM(CH) (12b)
DEDP(MM) = EMM(S�) � EMM(C�) � [EMM(SH) � EMM(CH)](12c)
If the cluster is large enough, the structural distortion upondeprotonation decays within the cluster region and theDEDP(MM) term consists only of electrostatic interactions, i.e.longrange contributions DELR.18 Hence,
DEDP = DEDP(QM) + DELR (13)
Effectively, the deprotonation energy of the whole system is thesum of the deprotonation energy of a cluster calculated at theQM level and the longrange term representing the electrostaticinteraction between the inner and the outer part of the system.This long range term is described at the MM level. Thus, thechoice of an appropriate force field is crucial for the success ofQM/MM calculations. To check if the applied embeddingscheme works correctly, the convergence of the deprotonationenergy with respect to the cluster size has to be investigated.
For the Leslie–Gillan method, with eqn (9) the total longrange correction, DEN
LR, is given by
DE1LR ¼ DELGDP � DEDP QMð Þ ¼ DELR �
E��eðLGÞ (14)
whereas for the supercell method it is obtained as
DEN
LR = DEN
DP � DEDP(QM) (15)
2.3 Details of QM/MM calculations
We used the QMPOT package,19,20 with DFT for the QM partand the DFTparametrized polarizable shell model potential ofSierka and Sauer21 for the MM part. The DFT calculationsof energies and forces were done using the TURBOMOLE22
package with the B3LYP functional and the TZVP basis setnamed ‘‘def2’’ in the TURBOMOLE library.23,24 The latterincludes the following contracted functions: H: (5s1p)/[3s1p],O: (11s6p2d1f)/[5s3p2d1f], and Si/Al: (14s9p3d1f)/[5s5p2d1f].The choice of functional is based on previous experiences,21,25
and motivated by the fact that deprotonation energies of smallaluminosilicate clusters calculated with the B3LYP functional
are in very good agreement with the CCSD(T) results (see TableS1 in the ESI†). For the shell model MM calculations, we usedthe GULP code,26 with parameters derived from B3LYP clustercalculations.21 It was shown21 that for this combination of QMand MM methods deprotonation energies of zeolites convergeto a constant value with increasing cluster size. This indicatesthat the polarizable shellmodel force field describes the electrostatic interactions as accurately as the B3LYP functional.
3. Results3.1 HCHA
The HCHA zeolite is chosen as a reference system because itconsists of hexagonal prisms as secondary building units likethe H2dH zeolite (Fig. 1).9 All tetrahedral atoms of HCHA arecrystallographically equivalent (Fig. 1) and there are only fourdistinct oxygen positions.28 The energies of structures with theproton attached to different oxygen positions are similar,25
therefore we calculate deprotonation energies for the lowestenergy structure only, i.e. with the proton attached to the O1oxygen. We used a unit cell consisting of 37 atoms,20,21 withHAlSi11O24 composition and cell parameters optimised usingthe shell model potential (see Table S2 in the ESI†). These unit
Fig. 1 Optimized 2 � 2 � 2 unit cell of HCHA zeolite together with thenumbering of oxygen atoms. The following colour scheme is adopted:silicon, oxygen, aluminium and hydrogen are depicted in yellow, red, greyand white, respectively. The pictures of molecular models were generatedusing the Jmol program.27
PCCP Paper
Ope
n A
cces
s A
rtic
le. P
ublis
hed
on 0
6 O
ctob
er 2
015.
Dow
nloa
ded
on 3
0/11
/201
5 10
:49:
30.
Thi
s ar
ticle
is li
cens
ed u
nder
a C
reat
ive
Com
mon
s A
ttrib
utio
n 3.
0 U
npor
ted
Lic
ence
.View Article Online
27876  Phys. Chem. Chem. Phys., 2015, 17, 2787327882 This journal is© the Owner Societies 2015
cell parameters were fixed during subsequent structure optimisation of protonated and deprotonated forms of the zeolite, forwhich we used the following convergence criteria: a maximumenergy change of 1 � 10�5 eV, a maximum gradient componentof 1 � 10�2 eV Å�1, and a maximum displacement componentof 1 � 10�3 Å. Cluster models of increasing size were generatedautomatically by selecting only those tetrahedral sites whichwere within a defined distance from the O1 site.
The QM clusters were always terminated with OH groupswith a fixed OH distance of 96.1 pm (Fig. 2). This is an equilibriumdistance that we obtained by free cluster optimization of similarcluster models.
To compare Leslie–Gillan deprotonation energies (eqn (9))with those obtained using the supercell method we performedcalculations for an embedded 8T12OH cluster model (eighttetrahedral sites terminated by 12 OH groups) with increasingsupercell size from 2 � 2 � 2 to 4 � 4 � 4. Fig. 3 and Table 1show that the corrected deprotonation energies of both methods,DE LG
DP and DE N
DP, agree within 0.6 kJ mol�1.The increase of DEDP(QM/MM) with increasing cell size is
perfectly compensated by the decrease of the aperiodic correction, E��/e(LG) (Leslie–Gillan method) or by the decrease of theA/hr��i, +B/hr��i3 correction term (supercell method) so thatthe DELG
DP and DEN
DP values, respectively, are perfectly convergedalready for the smallest 2 � 2 � 2 cell.
The dielectric constants calculated from the fitted parameters A and B (Fig. 3) and the average dielectric constantscalculated for the LG correction method from the shellmodel
potential are virtually identical. The variation of e(LG) with thecell size is less than 2%, with the cluster size (Table 2) beingslightly larger, 5%.
The QM part of the deprotonation energy is almost independentof the supercell size. This shows that the cluster structure is notaffected by the unit cell size and structural distortions do notextend beyond the 2 � 2 � 2 supercell. In absolute terms, the
Fig. 2 Cluster models applied in QM/MM calculations of the HCHA deprotonation energy.
Fig. 3 Uncorrected deprotonation energies of the 8T12OH cluster modelof HCHA embedded in N � N � N supercells (black dots). The solid line isthe fitting curve, eqn (8). Deprotonation energies corrected using the LGmethod (red triangles) as a function of the cubic root of the unit cellvolume and extrapolated deprotonation energy (dashed line).
Paper PCCP
Ope
n A
cces
s A
rtic
le. P
ublis
hed
on 0
6 O
ctob
er 2
015.
Dow
nloa
ded
on 3
0/11
/201
5 10
:49:
30.
Thi
s ar
ticle
is li
cens
ed u
nder
a C
reat
ive
Com
mon
s A
ttrib
utio
n 3.
0 U
npor
ted
Lic
ence
.View Article Online
This journal is© the Owner Societies 2015 Phys. Chem. Chem. Phys., 2015, 17, 2787327882  27877
charge–charge interaction, A/hr��i, is more than two orders ofmagnitude larger than the dipole–dipole aperiodic correctionterm, B/hr��i3 (Table 1). This supports the assumption of Leslieand Gillan that the aperiodic correction is given by the charge–charge interaction. We use the A/hr��i term only to correct allsubsequent deprotonation energies of the HCHA zeolite.
The results obtained with embedded clusters of increasingsize (Table 2) show that the corrected deprotonation energies ofthe HCHA zeolite converge to 1233 � 5 kJ mol�1. This energy isin very good agreement with the value of 1231 kJ mol�1,determined using the QM/MM methodology with a smallerbasis set,29 and with the value of 1235 kJ mol�1 obtained fromthe planewave DFT calculation with the BLYP functional (correctedfor the systematic error of the functional).29 A periodic planewaveDFT calculation with the PW91 functional yields a deprotonationenergy of 1176 kJ mol�1,30 but this value does not include theaperiodic correction and should be compared with our uncorrectedvalue, 1164 kJ mol�1. The remaining difference is small due todifferent basis sets and density functionals.
As we can see from Table 2, increasing the cluster sizedecreases the QM contribution of the deprotonation energyand simultaneously increases the total long range correction byalmost the same value. This shows that the force field describes
the electrostatic interaction consistent with the (B3LYP) functionalused for its parametrization. This has been documented beforefor Hartree–Fock calculations with correspondingly parametrized force fields.18 Geometric parameters of the acidic siteare not strongly affected by the size of the QM region, and theirvalues converge to constant values with increasing clustersize (see ESI,† Table S3). These all facts prove that the appliedQM/MM methodology is appropriate to describe the propertiesof zeolites. Therefore, it can be used to predict the deprotonationenergy of the H2dH system.
3.2 Ultrathin H2dH zeolite
To study the acidity of the ultrathin H2dH zeolite, we performed calculations for cells of HnAlnSi64�nO128 with increasingAl/Si ratio (Fig. 4), namely 1/63 (n = 1), 1/7 (n = 8) and 1/3(n = 16). The cells for the different Al/Si ratio have the same size,but correspond to 1 � 1, 2 � 2, and 2 � 2 supercells,respectively, because the size of the primitive cells differs.
Experimentally, twodimensional zeolites were prepared on aRu(0001) substrate.8,9,31 However the interaction between zeoliteand the substrate was found to be weak31 and we excluded theruthenium layer from our computational models. We applied 2Dperiodic boundary conditions and calculated electrostatic interactions using the Perry summation technique,32,33 implementedin the GULP code.26 This was necessary because for standard slabcalculations the energy of the charged system increases linearly withthe vacuum thickness, and diverges in the limit of infinite values.34
First, we optimized the unit cell parameters using the shellmodel potential, which were kept fixed during all subsequentcalculations. We prepared clusters of increasing size startingfrom a single hexagonal prism containing a Brønsted site (1D6Rmodel) and adding up to 6 adjoining hexagonal prisms formingthe 7D6R model (Fig. 5).
Table 1 Deprotonation energies (kJ mol�1) and their components for the8T12OH cluster model of HCHA embedded in different N � N � Nsupercells: DELG
DP and DEN
DP – deprotonation energies calculated usingthe Leslie–Gillan (LG) and supercell (SC) methods, respectively; DEDP(QM/
MM) and DEDP(QM) – (uncorrected) QM/MM deprotonation energy and itsQM part, respectively. Dielectric constants calculated as 1/3 of the trace ofthe dielectric constant matrix at the MM level (shellmodel potential) (LG),and calculated from eqn (10) using the fitted parameters A and B, andeeff(SC)
Unit cell 2 � 2 � 2 3 � 3 � 3 4 � 4 � 4
DELGDP 1238.0 1238.0 1238.0
E��/e(LG)a �37.6 �24.9 �18.6DEDP(QM/MM) 1200.4 1213.1 1219.4DEDP(QM) 1291.7 1292.4 1292.3DEN
DP 1238.6 1238.6 1238.6A/hr��ib �38.42 �25.61 �19.22B/hr��i3 b 0.22 0.07 0.02e(LG) 2.79 2.81 2.83eeff(SC) 2.75 2.74 2.74
a Eqn (9). b Eqn (10).
Table 2 Deprotonation energy components (kJ mol�1) for variousembedded cluster models of the HCHA zeolite embedded in a 2 � 2 �2 supercell. See Table 1 for definitions
Model DELGDP E��/e(LG)a DEDP DEDP(QM) DEN
LRb e(LG)
MM 1036.4 �34.0 1002.3 — — 3.098T12OH 1238.0 �37.6 1200.4 1291.7 �53.7 2.7912T12OH 1239.3 �36.1 1203.1 1276.4 �37.1 2.9116T16OH 1237.4 �36.8 1200.7 1290.7 �53.3 2.8633T34OH
c 1233.5 �24.7 1208.8 1267.3 �33.8 2.8344T34OH
c 1232.5 �24.0 1208.5 1267.1 �34.6 2.92
a Eqn (9). b Long range correction for LG corrected deprotonationenergy, see eqn (13). c Cluster models embedded in a 3 � 3 � 3supercell. Fig. 4 Optimized cells of the H2dH zeolite with different Al/Si ratios.
PCCP Paper
Ope
n A
cces
s A
rtic
le. P
ublis
hed
on 0
6 O
ctob
er 2
015.
Dow
nloa
ded
on 3
0/11
/201
5 10
:49:
30.
Thi
s ar
ticle
is li
cens
ed u
nder
a C
reat
ive
Com
mon
s A
ttrib
utio
n 3.
0 U
npor
ted
Lic
ence
.View Article Online
27878  Phys. Chem. Chem. Phys., 2015, 17, 2787327882 This journal is© the Owner Societies 2015
In some cases it was necessary to add some extra tetrahedralsites to avoid terminal O–H groups that are connected toneighbouring Brønsted sites. These additional Tsites areindicated by a subscript, e.g. 4D6R+4T stands for four additionaltetrahedral sites added to the 4DR6 cluster. Cluster modelswere terminated in the same way as for the HCHA zeolite.
The simple Leslie–Gillan method of aperiodic corrections isnot applicable to the H2dH system. For the twodimensionalcase, the macroscopic approximation is not valid anymore.To calculate corrected deprotonation energies for the H2dHzeolites, we used the supercell extrapolation method which iscomputationally demanding. The original unit cells were multiplied in 
a and
b directions and extrapolation curves, eqn (8),were fitted as a function of the square root of the surface area.A series of three supercells per each system, namely 1 � 1,2 � 2, and 3 � 3 for Al/Si = 1/63, and 2 � 2, 3 � 3, and 4 � 4 forAl/Si = 1/7 and 1/3, were used to extrapolate deprotonationenergies. All supercell structures were optimized, both theprotonated and deprotonated forms. The resulting fittingparameters and correction energies are presented in the ESI,†Table S4 and Fig. S3.
For each Al/Si ratio the fitted parameters A and (especially) Bdepend on the cluster model. Nevertheless, the correctionenergies, Ecorr (eqn (8)), are almost constant within 6 kJ mol�1.This means that one can calculate the aperiodic correctionenergy using the supercell approach for only one embeddedcluster model, or even at the MM level, and then apply thiscorrection for different embedded cluster models of the sameunit cell, tolerating an error of about 6 kJ mol�1.
The fitted A parameters are much larger for H2dH (ESI,†Table S4) than for HCHA (Fig. 3). This shows that in the twodimensional H2dH zeolite the interaction between chargeddefects is much less screened than that in the bulk HCHAzeolite. This is also reflected in very small effective dielectricconstants of H2dH, 1.5–1.8 (Table 3), compared to 2.9–3.1 forHCHA (Table 2).
The extrapolated deprotonation energies of the H2dHzeolites converge to constant values with increasing embedded
cluster size (Table 3 and ESI,† Fig. S4), which is also true for thegeometrical parameters of the Brønsted sites (see ESI,† TableS5). The deprotonation energies of all studied H2dH systemsare much lower than those of HCHA. Even the least acidic twodimensional system with Al/Si = 1/3 has a deprotonation energy(1091 kJ mol�1) which is 142 kJ mol�1 lower than that of HCHAwith Al/Si = 1/12.
Table 4 compares calculated deprotonation energies andtheir components for H2dH with different Al/Si ratios withthose for HCHA. The table shows that the QM part of thedeprotonation energy is significantly smaller for H2dH thanthat for HCHA. Nevertheless, the decisive factor for the verylow deprotonation energy of twodimensional zeolites is thelongrange term, which (in absolute terms) is a few times largerthan that for HCHA.
The longrange component of the deprotonation energyresults from the interactions between the inner part (clustermodel) and its periodic surroundings. Upon removing theproton there is a change in the electrostatic (Coulomb andpolarization) part of these interactions. The negative charge
Fig. 5 Cluster models applied in QM/MM calculations of the H2dHdeprotonation energy (Al/Si = 1/63, models for the other Al/Si ratios arepresented in Fig. S1 and S2 in the ESI†).
Table 3 Deprotonation energy components (kJ mol�1) calculated forvarious embedded cluster models of H2dH zeolites for different Al/Siratios using the supercell (SC) method
Al/Si Model DEN
DP DEQM DEN
LR Erel Ecorr(SC) eeff(SC)
1/63a MM 836.1 — — �184.3 �44.3 1.5291D6R 1032.1 1277.9 �245.8 �144.6 �42.9 1.5792D6R 1037.4 1244.7 �208.5 �139.9 �42.9 1.579b
3D6R 1041.0 1232.6 �182.0 �143.2 �45.3 1.4934D6R 1041.5 1227.2 �185.7 �137.5 �42.1 1.6075D6R 1042.8 1217.6 �174.9 �137.3 �42.1d 1.607d
6D6R 1044.8 1213.3 �168.7 �137.4 �42.1d 1.607d
7D6R 1045.0 1210.1 �165.1 �136.9 �42.1d 1.607d
1/7b MM 870.8 — — �191.3 �42.5 1.5911D6R+2T 1049.3 1320.4 �271.2 �142.5 �37.9 1.7812D6R+4T 1072.1 1249.2 �177.1 �137.2 �44.3 1.5233D6R+2T 1073.6 1238.3 �164.7 �137.8 �44.3e 1.523e
4D6R 1068.9 1235.9 �167.0 �135.8 �36.7 1.8407D6R+4T 1071.8 1229.4 �157.6 �134.5 �37.9 1.778
1/3c MM 890.3 — — �181.9 �41.8 1.5911D6R+4T 1069.6 1290.0 �220.4 �143.0 �41.3 1.6364D6R+4T 1090.6 1241.3 �150.7 �138.7 �43.0 1.570
a 2 � 2 cell, hr��i = 39.9 Å. b 4 � 4 cell, hr��i = 40.0 Å. c 4 � 4 cell,hr��i = 40.2 Å. d Ecorr(SC), and eeff(SC) taken from the 4R6 model.e Ecorr(SC), and eeff(SC) taken from the 2R6 model.
Table 4 Calculated deprotonation energies and their components(kJ mol�1) for twodimensional zeolites with different Al/Si ratios compared to HCHA
Systema Model DEN
DP DEDP(QM) DEN
LR Erel eeff(SC)
HCHA (1/11) 44T32OHb 1233 1267 �35 �144 2.92
H2dH (1/63) 4D6Rc 1042 1227 �186 �138 1.61H2dH (1/7) 4D6Rd 1069 1236 �167 �136 1.84H2dH (1/3) 4D6R+4T
c 1091 1241 �151 �139 1.57
a Al/Si ratio is in parentheses. b 3 � 3 � 3 unit cell. c 2 � 2 unit cell.d 4 � 4 unit cell.
Paper PCCP
Ope
n A
cces
s A
rtic
le. P
ublis
hed
on 0
6 O
ctob
er 2
015.
Dow
nloa
ded
on 3
0/11
/201
5 10
:49:
30.
Thi
s ar
ticle
is li
cens
ed u
nder
a C
reat
ive
Com
mon
s A
ttrib
utio
n 3.
0 U
npor
ted
Lic
ence
.View Article Online
This journal is© the Owner Societies 2015 Phys. Chem. Chem. Phys., 2015, 17, 2787327882  27879
created upon deprotonation is stabilized by its surroundings.This stabilization is maximum if there is no screening ofthe created charge (e = 1). The more efficient the screening(the larger e), the smaller is the electrostatic stabilization of thecreated charge. For the H2dH zeolites the dielectric constant isrelatively small, therefore the created charge is more stabilizedby the crystal field than the one in HCHA. If this interpretationis correct, one should observe a dependence of the deprotonationenergy of zeolites on their dielectric constant.
The geometric parameters of the Brønsted sites of H2dH(Al/Si = 1/63) and HCHA are almost the same (see ESI,† TablesS1 and S2) and the relaxation energies, Erel, of twodimensionaland bulk zeolites (Table 4) are also very similar. Both thesefacts confirm that differences in long range electrostatic interactions are indeed responsible for the observed differences indeprotonation energies.
3.3 Effect of the Al/Si ratio
The deprotonation energy of the H2dH zeolites increaseswith increasing Al/Si ratio (Table 4 and Fig. S4 in the ESI†).This behaviour was found in a number of experimental12,35,36
and theoretical studies.37–39 It suggests that an importantfactor governing the acidity of the Brønsted site is its localenvironment, i.e. the number of AlO4 tetrahedra in the secondcoordination sphere of the particular acidic site.12,35–38,40,41 Anincrease in the Al/Si ratio also affects the structure of theprotonated and the deprotonated Brønsted sites (Table S5 inthe ESI†), namely it decreases the Al–O bond length and theAl–O–Si angle and increases the Si–O bond length. Geometricparameters do not affect the relaxation energy of the anion,which is independent of the Al/Si ratio (Table 4). This suggeststhat the decrease of the acidity with increase of the Al content iscaused mainly by the changes of the electronic structure of thezeolite. In 3D zeolites this effect is localised,37,38 namely it iscaused by the interaction of the Brønsted site with its nearestsurroundings. However, comparison of the QM and long rangecontributions of the deprotonation energies of H2dH zeolites(Table 4) shows that the increase of the Al/Si ratio also affectsthe long range term.
3.4 Dielectric screening in twodimensional systems
The small dielectric constant of the H2dH thin film canbe explained by classical electrostatics, using the images.42
Let us first consider an electrostatic potential generated by apoint charge q immersed in a homogeneous dielectric film,characterised by a dielectric constant e1 and the thickness L,surrounded by a medium with a dielectric constant e2 (Fig. 6with e3 = e2).
The charge placed in the point (0, 0, a) generates thefollowing potential (in atomic units) at the point (x, 0, a):43
V2D x; a;Lð Þ ¼ q
e1
Xn¼1n¼�1
g nj jffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffix2 þ L
2� a� an
� �2s (16a)
With
g ¼ e1 � e2ð Þe1 þ e2ð Þ (16b)
an ¼ nLþ ð�1Þn L
2� a
� �(16c)
Let us now consider an electrostatic potential generated bythe point charge q immersed in the homogenous dielectricmedium of a bulk system, characterized by the dielectricconstant e. At a distance x from the charge the potential (inatomic units) is:
V3DðxÞ ¼q
ex(17)
By comparison of eqn (16a) and (17) we can determine theeffective dielectric constant eeff = e at the point (x, 0, a) of thedielectric slab:
eeff x; a;Lð Þ ¼ e1x
Xn¼1n¼�1
g nj jffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffix2 þ L
2� a� an
� �2s
0BBBB@
1CCCCA
�1
(18)
In contrast to bulk dielectrics, the effective dielectric constantof thin layers depends on the distance from the charge (Fig. 7).Independent of the sample’s thickness, the effective dielectricconstant on the surface (a = 0) changes continuously from (e1 +e2)/2 near the charge to e2 at an infinite distance from it (Fig. 7).In the case of the H2dH thin film, for which e1 (calculated as1/3 of the trace of the dielectric constant tensor, which wasdetermined from the shellmodel potential calculations) isabout 5 and e2 is equal to 1 (vacuum), the theoretical dielectricconstant should decrease from 3 near the charge to 1 at largedistances. During derivation of eqn (18) a few assumptionswere made, among others the assumption of homogenousdielectric medium and the assumption that the border betweentwo dielectric media is sharp. Nevertheless, the calculated dielectricconstant (1.6–1.9, Table 4) falls in the theoretical range (1 o eo 3),but a precise theoretical value cannot be specified.
We can use eqn (18) to predict the qualitative behaviour ofzeolite dielectric properties. For example, we know that theeffective dielectric constant depends on the distance a from the
Fig. 6 Model for dielectric constant calculations.
PCCP Paper
Ope
n A
cces
s A
rtic
le. P
ublis
hed
on 0
6 O
ctob
er 2
015.
Dow
nloa
ded
on 3
0/11
/201
5 10
:49:
30.
Thi
s ar
ticle
is li
cens
ed u
nder
a C
reat
ive
Com
mon
s A
ttrib
utio
n 3.
0 U
npor
ted
Lic
ence
.View Article Online
27880  Phys. Chem. Chem. Phys., 2015, 17, 2787327882 This journal is© the Owner Societies 2015
surface (Fig. 7). In other words, when e1 4 e2, increasing aincreases the dielectric constant. This is an important statementbecause it means that in the case of twodimensional zeolites wecannot compare uncorrected deprotonation energies of twodifferent Brønsted sites which are at different distances fromthe surface, even though the size of the unit cell is the same.This also suggests that the acidity of the Brønsted sites whichare deeper in the sample can be lower than of those which are atthe surface. The thickness of the sample changes the slope ofthe dielectric constant curve, namely with decrease of L thecurve becomes steeper (Fig. 7). Hence, we can expect that theacidity of the surface Brønsted sites should increase withdecrease of the sample thickness. To confirm these predictions,a separate study of the thickness dependence of deprotonationenergies for thin HMFI films6 is underway.
Let us consider the most general situation, namely a thinfilm characterized by a macroscopic dielectric constant e1
surrounded by different media at the top and the bottom withdielectric constants e2 and e3, respectively. This corresponds toour experimental model system, namely the ultrathin zeolitefilm deposited on the metal surface (e3 = N) under ultrahighvacuum conditions (e2 = 1.0). Once again we can apply themacroscopic approximation to calculate the electrostatic potential
within a film and subsequently the effective dielectric constant ofthe film.43 Fig. 8 shows the effective dielectric constant within thethin layer as a function of a distance x from the point charge,calculated for different dielectric constants of the bottom layer.The effective dielectric constant on the slab surface (a = 0)changes continuously from (e1 + e2)/2 near the charge to (e2 + e3)/2at large distances. It means that in the experimental case thedielectric screening near the charge is smaller than in the bulkzeolite, but for the bigger distances it quickly approachesinfinity. Therefore the long range interaction between the activesite and the crystal lattice should be much reduced with respectto the system without the metal substrate. If we assume thatthe influence of the metal substrate on the QM part of thedeprotonation energy is not strong (short range interaction) wecan expect that the acidity of the ultrathin zeolite adsorbedon the metallic surface should be reduced with respect to thefreestanding film.
3.5 Comparison with OH frequency shifts
Since deprotonation energies cannot be directly measured forsolid acids, a linear relationship has been suggested (Paukshtisand Yurchenko)44,45 between the OH frequency shift uponcomplex formation with a weak base molecule and the enthalpyof deprotonation, DHDP (kJ mol�1):
DHDP = 1390 � 442.5�log(D~nOH/D~nSiOH) (19)
Here, D~nOH and D~nSiOH are the wavenumber shifts for the O–Hstretching vibrations of Brønsted sites and free silanols, respectively(in cm�1), caused by the adsorption of weak bases. Because weare interested in the difference between two different zeolites,D(DEDP), we do not need to know D~nSiOH, which cancels out:
D(DEDP) E D(DHDP) = �442.5�log(D~nOH(H2dH)/D~nOH(HCHA))(20)
The wavenumber shifts upon CO adsorption from ref. 9, whichhave been calculated for exactly the same Si/Al = 7 bilayer asexamined in the present study, yield a deprotonation energy
Fig. 7 Theoretical effective dielectric constant (eqn (18)) as a function of adistance x from the charge calculated for e1 = 5.0 and e2 = 1.0 and differenta and L parameters.
Fig. 8 Theoretical effective dielectric constant as a function of a distancefrom the charge calculated for e1 = 5.0, e2 = 1.0, L = 5.3 Å, a = 0.0 Å anddifferent dielectric constants of the bottom layer (e3).
Paper PCCP
Ope
n A
cces
s A
rtic
le. P
ublis
hed
on 0
6 O
ctob
er 2
015.
Dow
nloa
ded
on 3
0/11
/201
5 10
:49:
30.
Thi
s ar
ticle
is li
cens
ed u
nder
a C
reat
ive
Com
mon
s A
ttrib
utio
n 3.
0 U
npor
ted
Lic
ence
.View Article Online
This journal is© the Owner Societies 2015 Phys. Chem. Chem. Phys., 2015, 17, 2787327882  27881
difference of only 12 kJ mol�1, one order of magnitude less thanthe calculated difference of 164 kJ mol�1 from Table 4. Insertionof experimental values of D~nOH(H2dH) and D~nOH(HCHA), 379and 316 cm�1, respectively,9 into eqn (20) yields a largerdeprotonation energy difference of 35 kJ mol�1, but which isstill much smaller than the calculated value of 164 kJ mol�1.
The obvious reason for the breakdown of the DHDP � D~nOH
plot is that the OH stretching frequency shift upon adsorptionof CO refers to an ‘‘early’’ stage of the reaction, whereasdeprotonation refers to a ‘‘late’’ stage of the catalytic reactionwhen the proton has been removed. This is consistent with thefinding that the much larger acidity ‘‘measured’’ with thedeprotonation energy is largely due to the better stabilizationof the created negative charge in media with low dielectricconstants such as twodimensional zeolites.
4. Conclusions
QM/MM calculations of deprotonation energies of ultrathinH2dH zeolites and the bulk HCHA zeolite confirm the muchhigher acidity of the ultrathin zeolites compared to bulksystems, previously observed in experiments.8,9 The very lowdeprotonation energy of the H2dH system reflects the factthat the dielectric constant of thin dielectrics immersed ina vacuum is much lower than that of corresponding bulksystems, resulting in a better stabilization of the charge createdupon deprotonation. The dielectric constant of a thin filmdepends on its thickness and on the distance of the chargefrom the surface. This suggests that the properties of acidicsites in ultrathin zeolites6,7 and single layer zeolites8,9 vary withtheir distance from the surface and can be tuned by changingthe sample’s thickness. Another consequence is that the acidityof twodimensional systems as judged upon deprotonationenergies is much larger than OH frequency shifts upon adsorptionof base molecules indicated.
Acknowledgements
This work has been supported by the German Research Foundation(DFG) through Collaborative Research Center Grant CRC 1109.The authors would like to thank Milan Oncak and RadosławWłodarczyk for helpful discussions.
References
1 A. Corma, Chem. Rev., 1995, 95, 559.2 A. Corma, J. Catal., 2003, 216, 298.3 W. O. Haag, R. M. Lago and P. B. Weisz, Nature, 1984, 309, 589.4 W. J. Mortier, J. Sauer, J. A. Lercher and H. Noller, J. Phys.
Chem., 1984, 88, 905.5 W. J. Roth, P. Nachtigall, R. E. Morris and J. Cejka, Chem.
Rev., 2014, 114, 4807.6 M. Choi, K. Na, J. Kim, Y. Sakamoto, O. Terasaki and
R. Ryoo, Nature, 2009, 461, 246.7 Y. Seo, K. Cho, Y. Jung and R. Ryoo, ACS Catal., 2013, 3, 713.
8 J. A. Boscoboinik, X. Yu, B. Yang, F. D. Fischer, R. Włodarczyk,M. Sierka, S. Shaikhutdinov, J. Sauer and H.J. Freund, Angew.Chem., Int. Ed., 2012, 51, 6005.
9 J. A. Boscoboinik, X. Yu, E. Emmez, B. Yang, S. Shaikhutdinov,F. D. Fischer, J. Sauer and H.J. Freund, J. Phys. Chem. C, 2013,117, 13547.
10 A. Zecchina, G. Spoto and S. Bordiga, Phys. Chem. Chem.Phys., 2005, 7, 1627.
11 J. Sauer, J. Mol. Catal., 1989, 54, 312.12 W. E. Farneth and R. J. Gorte, Chem. Rev., 1995, 95, 615.13 E. G. Derouane, J. C. Vedrine, R. R. Pinto, P. M. Borges,
L. Costa, M. A. N. D. A. Lemos, F. Lemos and F. R. Ribeiro,Catal. Rev., 2013, 55, 454.
14 J. E. Bartmess, J. A. Scott and R. T. McIver, Jr., J. Am. Chem.Soc., 1979, 101, 6046.
15 H. V. Brand, L. A. Curtiss and L. E. Iton, J. Phys. Chem., 1993,97, 12773.
16 M. Brandle and J. Sauer, J. Am. Chem. Soc., 1998, 120, 1556.17 M. Leslie and M. J. Gillan, J. Phys. C: Solid State Phys., 1985,
18, 973.18 U. Eichler, M. Brandle and J. Sauer, J. Phys. Chem. B, 1997,
101, 10035.19 U. Eichler, C. Kolmel and J. Sauer, J. Comput. Chem., 1997,
18, 463.20 M. Sierka and J. Sauer, J. Chem. Phys., 2000, 112, 6983.21 M. Sierka and J. Sauer, Faraday Discuss., 1997, 106, 41.22 TURBOMOLE V6.4; a development of the University
of Karlsruhe and Forschungszentrum Karlsruhe GmbH,http://www.turbomole.com, 2012.
23 F. Weigend, M. Haser, H. Patzelt and R. Ahlrichs, Chem.Phys. Lett., 1998, 294, 143.
24 F. Weigend and R. Ahlrichs, Phys. Chem. Chem. Phys., 2005,7, 3297.
25 M. Sierka and J. Sauer, J. Phys. Chem. B, 2001, 105, 1603.26 J. D. Gale, J. Chem. Soc., Faraday Trans., 1997, 93, 629.27 Jmol: an opensource Java viewer for chemical structures in
3D, http://www.jmol.org/.28 M. Calligaris, G. Nardin, L. Randaccio and P. C. Chiaramonti,
Acta Crystallogr., 1982, 38, 602.29 J. Sauer, K.P. Schroder and V. Termath, Collect. Czech.
Chem. Commun., 1998, 63, 1394.30 C. Lo and B. L. Trout, J. Catal., 2004, 227, 77.31 R. Włodarczyk, M. Sierka, J. Sauer, D. Loffler, J. J. Uhlrich,
X. Yu, B. Yang, I. M. N. Groot, S. Shaikhutdinov and H. J.Freund, Phys. Rev. B: Condens. Matter Mater. Phys., 2012,85, 085403.
32 D. E. Parry, Surf. Sci., 1975, 49, 433.33 D. E. Parry, Surf. Sci., 1976, 54, 195.34 E. Wasserman, J. R. Rustad and A. R. Felmy, Surf. Sci., 1999,
424, 19.35 H. Stach, J. Jaenchen, H. G. Jerschkewitz, U. Lohse, B. Parlitz
and M. Hunger, J. Phys. Chem., 1992, 96, 8480.36 B. Gil, E. Broclawik, J. Datka and J. Klinowski, J. Phys. Chem.,
1994, 98, 930.37 L. Grajciar, C. O. Arean, A. Pulido and P. Nachtigall, Phys.
Chem. Chem. Phys., 2010, 12, 1497.
PCCP Paper
Ope
n A
cces
s A
rtic
le. P
ublis
hed
on 0
6 O
ctob
er 2
015.
Dow
nloa
ded
on 3
0/11
/201
5 10
:49:
30.
Thi
s ar
ticle
is li
cens
ed u
nder
a C
reat
ive
Com
mon
s A
ttrib
utio
n 3.
0 U
npor
ted
Lic
ence
.View Article Online
27882  Phys. Chem. Chem. Phys., 2015, 17, 2787327882 This journal is© the Owner Societies 2015
38 M. Sierka, U. Eichler, J. Datka and J. Sauer, J. Phys. Chem. B,1998, 102, 6397.
39 A. G. Pel’menshchikov, E. A. Paukshtis, V. G. Stepanov,V. I. Pavlov, E. N. Yurchenko, K. G. Ione, G. M. Zhidomirovand S. Beran, J. Phys. Chem., 1989, 93, 6725.
40 G. M. Zhidomirov and V. B. Kazansky, in Advances inCatalysis, ed. D. D. Eley, H. Pines and P. B. Weisz, AcademicPress, 1986, vol. 34, p. 131.
41 J. Datka and B. Gil, J. Catal., 1994, 145, 372.42 J. Jackson, Classical Electrodynamics, Wiley, 3rd edn, 1998.43 M. Kumagai and T. Takagahara, Phys. Rev. B: Condens.
Matter Mater. Phys., 1989, 40, 12359.44 E. A. Paukshtis, R. I. Soltanov and E. N. Yurchenko, React.
Kinet. Catal. Lett., 1981, 16, 93.45 A. P. Evgenii and E. N. Yurchenko, Russ. Chem. Rev., 1983,
52, 242.
Paper PCCP
Ope
n A
cces
s A
rtic
le. P
ublis
hed
on 0
6 O
ctob
er 2
015.
Dow
nloa
ded
on 3
0/11
/201
5 10
:49:
30.
Thi
s ar
ticle
is li
cens
ed u
nder
a C
reat
ive
Com
mon
s A
ttrib
utio
n 3.
0 U
npor
ted
Lic
ence
.View Article Online